Concrete Components • Cement • Water • Fine Aggregate • Coarse Aggregate
Advantages of Reducing Water Content: • Increased strength • Lower permeability • Increased resistance to weathering • Better bond between concrete and reinforcement • Reduced drying shrinkage and cracking • Less volume change from wetting and drying
Workability — that property of freshly mixed concrete that determines its working characteristics ie. the ease with which it can be mixed, placed, compacted and finished.
Cross Section of Hardened Concrete Concrete made with siliceous rounded gravel Concrete made with crushed limestone
Factors Affecting Workability • Method and duration of transportation • Quantity and characteristics of cementing materials • Concrete consistency (slump) • Agg. grading, shape & surface texture • % entrained air • Water content • Concrete & ambient air temperature • Admixtures
Effect of Voids in Concrete on Modulus of Elasticity, Compressive Strength, and Flexural Strength.
Hydration ─ is the chemical reaction between the cement and water in which new compounds with strength producing properties are formed. Heat of Hydration ─ is the heat given off during the chemical reaction as the cement hydrates.
Curing ─ maintenance of a satisfactory moisture content and temperature in concrete for a suitable period of time immediately following placing & finishing so that the desired properties may develop. • Time • Temperature • Moisture
Concrete Strength Gain Versus Time for Concrete Exposed to Outdoor Conditions
Drying Shrinkage and Mass Loss of 150 x 300-mm Cylinders Moist Cured for 7 days
— is defined as the measured maximum resistance of a concrete or mortar specimen to an axial load, usually expressed in MPa at an age of 28-days. Compressive Strength • Most general use concrete 20 to 40 MPa • High-strength concrete by definition 70 MPa or greater
Compressive Strength Test Specimen SizesCSA A23.1-00 • Mortar — 50 mm cubes • Concrete — 100 x 200 mm cylinders* *(generally 150 x 300 mm in USA)
Ratios — W/CM and W/C • Water-cementing materials ratio (w/cm) — ratio of mass of water to mass of cementing materials in a concrete mix expressed as a decimal. The water is exclusive to that absorbed by the agg. • Water-cement ratio (w/c) — ratio of mass of water to mass of cement in a concrete mix expressed as a decimal.
Approximations of Concrete Strengths • Compressive strength ( ƒc′ ) 7-day — 75% of 28-day 56 and 90-day — 10% - 15% > 28-day • Flexural Strength ( Modulus of Rupture) normal density — 8% - 12% of ƒc′ • Tensile Strength direct tensile — 8% -12% of ƒc′ splitting tensile — 8% -14% of ƒc′
E and DensityApproximate Values • Modulus of Elasticity ( E ) normal concrete — 14,000 to 41,000 MPa • Density normal concrete — 2200 to 2400 kg/m3 reinforced concrete — 2400 kg/m3 low density insulating concrete — 240 kg/m3 high density concrete — 6000 kg/m3 (radiation shielding, counterweights)
Watertightness / Permeability • Watertightness — the ability of concrete to hold back or retain water without visible leakage. • Permeability — amount of water migration through concrete when the water is under pressure or the ability of concrete to resist penetration by water or other substances (liquids, gas, ions, etc.)
Relationship between Hydraulic Permeability, W/C-Ratio, and Initial Curing
Effect of W/C-Ratio and Air Content on the Total Charge at the End of the Rapid Chloride Permeability Test
Effect of Compressive Strength and Aggregate Type on the Abrasion Resistance of Concrete
Effect of Hard Steel Troweling and Surface Treatments on the Abrasion Resistance of Concrete (ASTM C 779)
Non-air-entrained High water-cement ratio Specimens subjected to 150 Cycles of Freezing and Thawing • Air-entrained • Low water-cement ratio
Type 10 cement Relationship Between Freeze-Thaw Resistance, W/C- Ratio, and Different Concretes and Curing Conditions (1)
Type 10 cement Relationship Between Freeze-Thaw Resistance, W/C- Ratio, and Different Concretes and Curing Conditions (2)
Alkali- Aggregate Reactivity ( AAR ) • — is a reaction between the active mineral constituents of some aggregates and the sodium and potassium alkali hydroxides and calcium hydroxide in the concrete. • Alkali-Silica Reaction ( ASR ) • Alkali-Carbonate Reaction ( ACR ) Refer CSA A23.1-00 Appendix B — Alkali-Aggregate Reaction
Alkali-Silica Reactivity ( ASR ) • Control ASR with: • SCM’s • Blended cement • Limit concrete alkali content • Test for effectiveness
Methods to Reduce Corrosion of Embedded Steel by Chlorides • Use low w/cm ratio concrete • Moist cure • Reduce permeability with SCM’s • Increase concrete cover • Corrosion inhibitors • Epoxy-coated reinforcing steel • Concrete overlays • Surface treatments • Cathodic protection
Sulphate Attack • Use low w/cm (ie. 0.4) • Use sulphate resistant cement
Concrete Beams After Seven Years of Exposure to Sulphate-Rich Wet Soil